Accepted Manuscript Comparison of Antibacterial activities of Ag@TiO2 and Ag@SiO2 Core - Shell Nanoparticles K.I. Dhanalekshmi, K.S. Meena PII: DOI: Reference:
S1386-1425(14)00250-9 http://dx.doi.org/10.1016/j.saa.2014.02.063 SAA 11694
To appear in:
Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy
Received Date: Revised Date: Accepted Date:
21 November 2013 5 February 2014 14 February 2014
Please cite this article as: K.I. Dhanalekshmi, K.S. Meena, Comparison of Antibacterial activities of Ag@TiO2 and Ag@SiO2 Core - Shell Nanoparticles, Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy (2014), doi: http://dx.doi.org/10.1016/j.saa.2014.02.063
This is a PDF file of an unedited manuscript that has been accepted for publication. As a service to our customers we are providing this early version of the manuscript. The manuscript will undergo copyediting, typesetting, and review of the resulting proof before it is published in its final form. Please note that during the production process errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain.
Comparison of Antibacterial activities of Ag@TiO2 and Ag@SiO2 Core - Shell Nanoparticles K. I. Dhanalekshmi, Dr. K. S. Meena PG & Research Department of Chemistry, Queen Mary’s College, Chennai-600 004, Tamil Nadu, India. [email protected]
Abstract Core-shell type Ag@TiO2 nanoparticles were prepared by one pot simultaneous reduction of AgNO3 and hydrolysis of Ti (IV) isopropoxide and Ag@SiO2 core-shell nanoparticles were prepared by Stober’s method. They were characterized by absorption, XRD, and HR-TEM techniques. XRD patterns show the presence of anatase form of TiO2 and amorphous form of SiO2 and the noble metal (Ag). High resolution transmission electron microscopy measurements revealed that their size is below 50 nm. The antibacterial properties of Ag@TiO2 and Ag@SiO2 core-shell nanoparticles against Escherichia coli (E. coli) and Staphylococcus aureus (S. aureus) were examined by the agar diffusion method. As a result E. coli and S. aureus were shown to be substantially inhibited by Ag@TiO2 and Ag@SiO2 core-shell nanoparticles. These results demonstrated that TiO2 and SiO2 supported on the surface of Ag NPs without aggregation was proved to have enhanced antibacterial activity. Keywords: Core- shell nanoparticles, Escherichia coli, Staphylococcus aureus, Antibacterial activity. 1. Introduction Antibacterial activity agents are very important in the textile industry , water disinfection, medicine and food packaging. Organic compounds used for disinfection have some disadvantages, including toxicity to the human body, therefore the interest in inorganic disinfectants such as metal oxide nanoparticles is increasing . Inorganic antibacterial agents are superior to organic antibacterial materials in terms of their durability , heat resistance, toxicity, selectivity and various other characteristics . Among the inorganic nanoparticles, silver has been recognized as an effective antimicrobial agent that exhibit low toxicity in human and has diverse in vitro and in vivo application . Ag nanoparticles have attracted considerable attention and have been used as an antibacterial activity and the unlikeness to develop resistant microorganisms [4,5]. The principal characteristic of Ag nanoparticles is their high surface area to volume ratio, resulting in the appearance of new mechanical , chemical, electrical, optical, magnetic, electro-optical, and magneto-optical properties of the nanoparticles that are different from their bulk properties . The antimicrobial of activity of Ag nanoparticles is the result of the interaction of silver ions with the three main components of the bacterial cell: the peptidoglycan cell wall and plasma membrane , bacterial DNA and bacterial protein, particularly enzymes . It is widely believed 1
that silver nanoparticles are incorporated into the cell membrane, which cause leakage of intracellular substances and eventually causes cell death [8,9]. Some of the silver nanoparticles incorporated, also penetrate into the cells. The antimicrobial activity increases with decreasing size of the Ag nanoparticles . But Ag nanoparticles with diameters less than 200 mm tend to aggregate spontaneously, and their stability in air, water, or sunlight is not good enough for long term applications , which will decrease their antibacterial performance. To solve this problem , a wide range of materials TiO2 , SiO2 , Al2O3 , zeolites  and activated carbon fibers  have been employed to support Ag nanoparticles, so that the ultra fine Ag nanoparticles can be homogeneously formed without aggregation . Among the various oxide semiconductors , TiO2 and SiO2 have proven to be the most suitable for widespread environment application for its high chemical stability, non-toxicity , low cost and excellent degradation of organic pollutants [18-22]. The core-shell composite structures , as a kind of new nanostructures, have received intense attention due to their improved physical and chemical properties over their single components, and thus many efforts have been made to synthesize such special core-shell nanostructures [23,24]. The core-shell composite has many advantages as antibacterial agent, such as high antibacterial activity, low toxicity, chemical stability, long lasting action period and thermal resistance versus organic antibacterial agents . The Ag core-shell nanoparticles would provide a new possibility to be good candidates for antibacterial materials due to their unique structures and at the same time the shell to protect Ag nanoparticles and stabilize them against chemical corrosion. It could be reasonably envisioned that Ag cores would release Ag ion slowly through the outer porous coating layer , thereby producing and maintaining the excellent antibacterial effects . Hence the present study is aimed to synthesize the core-shell type Ag@TiO2 and Ag@SiO2 NPs , characterize them and compare their antibacterial activity in vitro. 2. Materials and Methods 2.1. Reagents Titanium (iv) isopropoxide and tetraethoxysilane (TEOS) were purchased from Sigma Aldrich. AgNO3 was obtained from Merck and all the other chemicals used were of Analar grade. The water used to be of Milli–Q type. 2.2. Synthesis of Ag@TiO2 core-shell nanoparticles The core-shell type Ag@ TiO2 was prepared by slight modification of the method described in the literature . In brief 20 mM each of Ti (IV) isopropoxide and acetylacetone in 30ml of isopropanol was prepared by sonicating the mixture for 15 minutes. 10 mM solutions of AgNO3 in 5ml of milli-Q water was prepared and 20ml of DMF was added to it and stirred well. To this solution 30ml of the above sonicated solution was added and stirring continued for 10 2
more minutes. The final mixture was refluxed between 60 - 70°C for 1 hour. The solution became greenish black and the refluxing was continued for 1 more hour. The precipitate obtained was sonicated for 2 hours to disperse. On adding toluene the colloidal material was precipitated and washed several times with toluene and redissolved in isopropanol. The solvent was evaporated at room temperature to get a greenish black powder of Ag@TiO2 core –shell nanoparticles. 2.3. Synthesis of Ag@SiO2 core-shell nanoparticles Silica particles were prepared by adding dropwise the mixture of 18ml of ethanol and 6ml TEOS to the mixture of 42ml ethanol and 9ml NH4OH (25% NH3) under constant stirring. The titration speed was controlled at 20 seconds per droplet and after the titration , the stirring was performed continuously for 1 hour. The obtained silica colloid was aged for 1 day and no purification treatment was carried out. 7.5ml of the one-day-old silica colloid was mixed with a water-ethanol (1:9) solution containing 0.3mmol AgNO3 with stirring. A dilute ethanol solution containing excessive formaldehyde was added dropwise at a titration speed of 14 seconds per droplet under constant stirring. The obtained yellow solution was aged for 1 day and then was centrifuged and washed with water three cycles to remove residual reactants. 2.4. Characterization UV–visible spectra were recorded in a spectrophotometer (Perkin Elmer Lambda 35). X-ray diffraction (XRD) patterns were taken from X’pert PRO PANalytical diffractometer operating with CuK ( radiation (λ=1. 5406A°) source. High resolution transmission electron microscopy (HRTEM)
photographs were taken using a JEOL JEM -3010 Electron microscope operating at 300 keV. The magnifying power used was 600 and 800k times. 2.5. Antibacterial activity test The in vitro antibacterial activity of Ag@TiO2 and Ag@SiO2 core-shell NPs were tested against the bacterial species S. aureus, and E. coli by agar diffusion method . Initially, the stock cultures of bacteria were revived by inoculating in broth media and grown at 37 ºC for 18 hrs. The agar plates of media (peptone-10 g, NaCl-10 g and yeast extract 5 g, agar 20 g in 1000 ml of distilled water) were prepared and wells were made in the plate. Each plate was inoculated with 18 h old cultures (100 µl) and spread evenly on the plate. After 20 minutes, the wells were filled with compound at 100, 200,300,400,500 and 600 µg/ml concentrations, to determine the minimum inhibitory concentration (MIC) value. All the plates were incubated at 37 ºC for 24 h and the diameter of inhibition zone were noted.
3. Results and Discussion 3.1.UV-Visible spectral analysis The absorption spectrum of Ag@TiO2 is shown in Fig.1. It has a broad band centered at 425nm. The absorption spectrum of Ag@SiO2 is shown in Fig.2. It has a narrow band centered at 405nm.The red shift observed with respect to the Ag core metals in both cases may be due to increase in the particle dimension and /or dielectric constant of the surrounding matrix upon encapsulation . 3.2. XRD Analysis Standard X-ray powder diffraction was used to determine the identity, relative proportion and average grain size of the core-shell nanoparticles. Fig. (3a & 3b) shows the X-ray diffraction pattern of pre and post annealed Ag@TiO2 (at 650°C in the air for 5hrs) respectively. The Figure 3 (a) shows that the air dried Ag@TiO2 core-shell nanoparticle is fully amorphous since there is no peak corresponding to TiO2 and Ag. The Fig 2 (b) shows 4 characteristic peaks of nanocrystalline pure Ag@TiO2 of monoclinic structure. The major diffraction intensity peaks at 2θ, about 25.42, 32.182, 37.995, 47.839° were identified to originate from (220), (420) (112) and (040) planes of Ag@TiO2 respectively. Fig (4a & 4b) shows the x-ray diffraction pattern of pre and post annealed Ag@SiO2 (at 650°C in the air for 5hrs) respectively. The Fig.3a shows that the air dried Ag@SiO2 core-shell nanoparticles is fully amorphous since there is no peak corresponding to SiO2 and Ag. Fig.3b shows four distinct characteristic peaks observed at 2θ values of 38.15, 44.35, 64.45, 77.40o were indexed as (111), (200), (220) and (311) which are typical of a face centered cubic structure of silver. No peak assigned to silica crystal appeared, suggesting that the silica shell was amorphous.
3.3. High resolution scanning electron microscopy (HR-TEM) The HR-TEM images of Ag@TiO2 are shown in Fig.S1. The images show a majority of dark images of Ag core in the size regime. Fig.S1. illustrates the formation of nearly spherical particles of silver core with a particle diameter of 15nm to 20nm and a range of particle morphologies are seen. Although most of the particles seen in this image are spherical or oval, faceted structures were also observed. All of them appear to be associated with TiO2 shell. The HR-TEM images of Ag@SiO2 are shown in Fig.S2. nearly well defined spherical morphology is observed. Its sizes distribute between 20 to 50nm with an average of about 42nm. The shell thickness is found to be 37nm.This image illustrates that each particle has a thin capping of SiO2 shell.
3.4. Comparison of Antibacterial activity: The inhibition zone values were determined for Ag@TiO2 and Ag@SiO2 core-shell NPs were tested against two types of bacteria E.coli and S.aureus results are shown in the Fig.S3a & b. The MIC observed in this study for Ag@TiO2 core-shell NPs are 200 µg/ml for E. coil and 100 µg/ml for S. aureus and Ag@SiO2 core-shell NPs are 100 µg/ml for both E. coli and S. aureus. Comparing the antibacterial activity for the same concentration of nano-photosensitizers Ag@SiO2 has higher antibacterial activity than Ag@TiO2. The bacterial effect of NPs depends on the high surface area, which allows them to interact closely with microbial membranes . The surface area of SiO2 is larger than the TiO2. Hence Ag@SiO2 shows higher antibacterial activity. The obtained data demonstrate that all the investigated core-shell NPs had relatively high antibacterial activity against Gram negative (E. coli) bacteria as compared to that of Gram positive (S. aureus) bacteria. The antibacterial activity increases as the concentration of coreshell increases. The inhibition zone of S.aureus is smaller than that for E.coli. It has been known , that the structure of gram positive and gram negative cell walls has different compositions. The layer of peptidoglycan in gram positive bacteria is thicker than for gram negative bacteria which consequently decrease the penetrations of NPs to the cell wall of gram positive bacteria. Ag NPs shows three different ways of mechanism of action. Firstly , Ag NPs attaches to the surface of the cell membrane and disturb its power functions. Such as permeability and respiration . It is reasonable to state that the binding of the particles to the bacteria depends on the interaction of the surface area available. Secondly Ag NPs are able to penetrate the bacteria and came further damage, possibly by interacting with sulfur and phosphorus containing compounds such as DNA . In addition , it is believed that Ag NPs after penetration into the bacteria have inactivated their enzymes, generating hydrogen peroxide and causing bacterial cell death [31,32]. Third , Ag NPs release silver ions, which made an additional contribution to the bactericidal effect . The Ag NPs also contain micro molar concentration of Ag+ and they have shown that Ag+ and Ag0 both contribute to the antibacterial activity. The mechanism of inhibition by silver ions on micro organisms in partially known. It is believed that DNA loses its replication ability and cellular proteins become inactivated on silver ion treatment . Higher concentrations of Ag+ ions have been shown to interact with cytoplasmic components and nucleic acids . It could be concluded that Ag ions from Ag cores could be released through porous TiO2 and SiO2 shells. It may be reasonable to presume that such core/shell structures will benefit 5
preventing corrosion and prolonging the release time of Ag ions and preserving the sustained antibacterial behavior . Therefore such Ag@TiO2 and Ag@SiO2 core-shell nanoparticles could be useful and effective in bactericidal applications, and would present a reasonable alternative for the development of new bactericides. 4. Conclusion: Ag@TiO2 and Ag@SiO2 core-shell nanoparticles were successfully prepared and their structure was analyzed by techniques such as UV-Vis spectroscopy, XRD and HR-TEM. The antibacterial activity of Ag@SiO2 is higher than the Ag@TiO2 due to their larger surface area. Positively charged silver reacted easily with gram negative bacteria rather than gram positive bacteria. They could be more effectively killed by the Ag@SiO2 rather than Ag@TiO2 core-shell NPs. The core-shell NPs showed good antibacterial activities because of TiO2 and SiO2 deposited on the surface of Ag NPs which prevents aggregation. Such core-shell NPs could have promising application as antibacterial materials for microbiocides and in water treatment. References:  Hajipour et al, Antibacterial properties of nanoparticles, Trends in Biotechnology, doi:10.1016/j.tibtech2012.06.004,2012.  Q.X.Li , H.A.Tang, Y.Z.Li, M.Wang, L.F.Wang, C.G.Xia, J.Inorg.Biochem.78 (2000) 167-174.  Farooqui, M.D.A, Chauhan, P.S., Krishanmoorthy, P and Shaik ,J .Extraction of Ag Nanoparticles from the leaf extracts of Clerodendrum inerme, Digest Journal of nanomaterials and biostructures, 2010; 5:43-49.  V.K.Sharma, R.A.Yngard, Y.Lin, Silver nanoparticles: green synthesis and their antimicrobial activites, Advances in colloid and Interface Science 145 (2009) 83-96.  Q.Li, S. Mahaendra, D.Y. Lyon, l. Brunet, M.V. Liga, D. Li, P.J.J. Alvarez, Antimicrobial nanomaterials for water disinfection and microbial control: potential applications and implications, Water research 42 (2008) 4591-4602.  Whitesides, G.M. (2005) Nanoscience, nanotechnology, and chemistry. Small 1,172-179.  K. Chaloupka , Y. Malam, A.M. Seifalian, Trends Biotechnol.28 (2010) 580.  Sondi I, Salopek-Sondi B. Silver nanoparticles as antimicrobial agent: a case study on E. Coli as a model for gram- negative bacteria. J. Colloid Interf Sci-2004; 223:313-9.  Cho K, Park J, Osaka T, Park S. The study of antimicrobial activity and preservative effects of nanosilver ingredient. Electrochim Acta 2005;51:5255-62.  C. Baker, A. Pradhan, L. Pakstis, D.J. Pochan, S.I. Shah, J. Nanosci. Nanotechnol.5 (2005) 244.  Shunsheng Cao, Juanrong Chen, Jie Hu, Aust. J. Chem. 62 (2009) 1561-1576.  O. Akhavan, Lasting antibacterial activities of Ag–TiO2/Ag/a-TiO2 nanocomposite thin 6
film photocatalysts under solar light irradiation, J. Colloid Interface Sci.336 (2009) 117–124.  S.D. Oh, S.H. Lee, S.H. Choi, I.S. Lee, Y.M. Lee, J.H. Chun, H.J. Park, Synthesis of Ag and Ag–SiO2 nanoparticles by irradiation and their antibacterial and antifungal efficiency against Salmonella enterica serovar Typhimurium and Botrytiscinerea, Colloids Surf. A: Physicochem. Eng. Aspects 275 (2006) 228–233.  Q.Y. Chang, L.Z. Yan, M.X. Chen, H. He, J.H. Qu, Bactericidal mechanism of Ag/Al2O3 against Escherichia coli, Langmuir 23 (2007) 11197–11199.  Y. Inoue, M. Hoshino, H. Takahashi, T. Noguchi, T. Murata, Y. Kanzaki, H. Hamashima, M. Sasatsu, Bactericidal activity of Ag–zeolite mediated by reactive oxygen species under aerated conditions, J. Inorg. Biochem. 92 (2002) 37–42.  S.X. Chen, J.R. Liu, H.M. Zeng, Structure and Antibacterial activity of silver supporting activated carbon fibers, J. Mater. Sci. 40 (2005) 6223–6231.  Y.H. Kim, D.K. Lee, H.G. Cha, C.W. Kim, Y.S. Kang, Synthesis and characterization of antibacterial Ag–SiO2 nanocomposite, J. Phys. Chem. C 111 (2007), 3629–3635.  M. Ksibi, S. Rossignol, J.M. Tatibouet, C. Trapalis, Synthesis and solid characterization of nitrogen and sulfur-doped TiO2 photocatalysts active under near visible light, Mater. Let. 62 (2008) 4204–4206.  W.P. Wang, J.L. Zhang, F. Cheng, D. He, M. Anpo, Preparation and photocatalytic properties of Fe3+-doped Ag@TiO2 core–shell nanoparticles, J. Colloid Interf. Sci. 323 (2008) 182–186.  Q.H. Zhang, W.G. Fan, L. Gao, Anatase TiO2 nanoparticles immobilized on ZnO tetrapods as a highly efficient and easily recyclable photocatalyst, Appl. Catal. B 76 (2007) 168–173.  J.G. Yu, X.J. Zhao, Q.N. Zhao, Effect of surface structure on photocatalytic activity of TiO2 thin films prepared by the sol – gel method, Thin Solid Films 379 (2000) 7–14.  R. Fan, Y.Wu, D. Li, M. Yue, A. Majumdar. P. Yang, fabrication of silica nanotube arrays from vertical silicon nanowire template technique, Adv. Mater. 15(2003) 5254.  M.E. Ahmed, Y. Shu, S. Tsugio, J. Colloid Interface sci. 300 (2006) 123.  M. Bonini, a. Wiedenmann, P. Baglioni, Mater. Sci. Eng. C26 (2006) 745.  E.C. Antonio, P. Carlos, A. Eduardo, S. Julio, M.J. Antibacte. J. Mater. Sci.41 (2006) 5208.  Yue lin, Wang Qiqiang, Zhang Xiaoming, Wang Zhouping, Xia Wenshui, and Dong Yuming. Bull. Korean Chem. Soc. 2011, Vol.32, No. 2607.  T. Renjis, A. Tom, SreeKumaran Nair, M. Navinder Singh, Aslam, C.L. Nagendra, Reji Philip, K. Vijaya Mohanan and T. Pradeep, Freely Dispersible Au@TiO2, Au@ZrO2 ; Ag@TiO2 and Ag@ZrO2 Core-Shell Nanoparticles: One-Step Synthesis, Characterization Spectroscopy and Optical Limiting Properties. Langmuir, 19, (2003), 3439-3445.  E. J. Threlfall, I. S. T. Fisher, L. Ward, H. Tschape, P. Gernersmidt, Microb. Drug Resist.5 (1999) 195-199.  Morones JR, Elechiguerra JL, Camacho A, Hoct K, Kouri JB, Ramirez JT et al. The bactericidal effect of silver nanoparticles. Nanotechnology 2005; 16: 2346-53.  Murray, R. G. E., Steed, P. & Elson, H. E. (1965) ,The location of the mucopeptide in 7
sections of the cell wall of Escherichia coli and other gram negative bacteria, Can. J. Microbiol. 11, 547-560.  M. Raffi, F. Hussain, T. M. Bhatti, J. I. Akhter, A. Hameed, M. M. Hasan, J. Mater. Sci. Technol. 24, 192 (2008).  Shockman GD, Barrett JF, Structure , function and assembly of cell walls of gram +ive bacteria. Annu Rev. Microbial, 1983:37:501-27.  Feng et.al , A mechanistic study of the a.bact effect of Ag ions on E.coli and S.aureus. 2000,662-668.  P. Gupta , M. Bajpai and S. K. Bajpai. Investigation of Antibacterial Properties of Silver Nanoparticle-loaded Poly (acrylamide-co-itaconic acid) -Grafted Cotton Fabric. The Journal of Cotton Science 12:280–286 (2008).  Lin et al Synthesis of Ag@TiO2 core-shell nanoparticles with antibacterial properties, Bul. Korean Chem.. Soc. 2011, Vol.32, No.8, 2607.
Fig.1. UV-Vis spectra of Ag@TiO2 core-shell NPs
Fig.2. UV-Vis spectra of Ag@SiO2 core-shell NPs
Fig.3. XRD spectrum of Ag@TiO2 core-shell NPs a) air dried sample and b) sample annealed at 650 0 C
Fig.4. XRD spectrum of Ag@SiO2 core-shell NPs a) air dried sample and b) sample annealed at 650 0 C
Core-shell type Ag@TiO2 nanoparticles were prepared by one pot simultaneous reduction of AgNO3 and hydrolysis of Ti(IV) isopropoxide and Ag@SiO2 core-shell nanoparticles were prepared by Stober’s method. The antibacterial properties of Ag@TiO2 and Ag@SiO2 core-shell nanoparticles against Escherichia coli (E.Coli) and Staphylococcus aureus (S.aureus) were examined by the agar diffusion method. Comparing the antibacterial activity for the same concentration of nano-photosensitizers Ag@SiO2 has higher antibacterial activity than Ag@TiO2. The obtained data demonstrates that all the investigated core-shell NPs had relatively high antibacterial activity against Gram negative (E.coli) bacteria as compared to that of Gram positive (S.aureus) bacteria